##############################################################################
###                                                                        ###
###        Electronic paper (Acta Crystallographica Section E)             ###
###                                                                        ###
##############################################################################
#                                                                            #
# This CIF contains the data in a paper accepted for publication in Acta     #
# Crystallographica Section E. It conforms to the requirements of Notes      #
# for Authors for Section E, and has been peer reviewed under the auspices   #
# of the IUCr Commission on Journals.                                        #
#                                                                            #
# Full details of the Crystallographic Information File format               #
# are given in the paper "The Crystallographic Information File (CIF):       #
# a New Standard Archive File for Crystallography" by S. R. Hall, F. H.      #
# Allen and I. D. Brown [Acta Cryst. (1991), A47, 655-685].                  #
#                                                                            #
# The current version of the core CIF dictionary is obtainable from          #
# ftp://ftp.iucr.org/pub/cif_core.dic. The current version number is 2.1.    #
#                                                                            #
# Software is freely available for graphical display of the structure(s) in  #
# this CIF.  For information consult the CIF home page http://www.iucr.org/  #
# cif/home.html                                                              #
#                                                                            #
#            Copyright International Union of Crystallography                #
#                                                                            #
##############################################################################
                                             
data_global
_audit_creation_method     from_MolEN_master_file_using_cif_in
_journal_date_recd_electronic     2001-04-19
_journal_date_accepted     2001-04-27
_journal_name_full     'Acta Crystallographica, Section E'
_journal_year     2001
_journal_volume     57
_journal_issue      6
_journal_page_first     i46
_journal_page_last     i48
_journal_paper_category     EI
_publ_contact_author_name     'P. Gougeon'
_publ_contact_author_address
;
Laboratoire de Chimie du Solide et Inorganique Moleculaire
UMR CNRS No. 6511
Universite de Rennes I
Avenue du General Leclerc
35042 Rennes CEDEX
France
;
_publ_contact_author_email     patrick.gougeon@univ-rennes1.fr
_publ_contact_author_fax     '(33) 99 63 57 04'
_publ_contact_author_phone     '(33) 99 28 62 54'
_publ_section_title
;
NdMo~7.7~O₁₄ containing Mo₆, Mo₇ and Mo₈ clusters
;
loop_
    _publ_author_name
    _publ_author_address
    'Barrier, N.'
;
Laboratoire de Chimie du Solide et Inorganique Moléculaire
URA CNRS No. 6511
Université de Rennes I
Avenue du Général Leclerc
35042 Rennes CEDEX
France
;
    'Gougeon, P.'
;
Laboratoire de Chimie du Solide et Inorganique Moléculaire
URA CNRS No. 6511
Université de Rennes I
Avenue du Général Leclerc
35042 Rennes CEDEX
France
;
data_nd
_audit_creation_method     SHELXL-97
_chemical_name_systematic
;
?
;
_chemical_name_common     ?
_chemical_formula_moiety     'Nd Mo7.70 O14'
_chemical_formula_sum     'Mo7.70 Nd O14'
_chemical_formula_iupac     'Nd Mo7.70 O14'
_chemical_formula_weight     1106.98
_chemical_melting_point     ?
_symmetry_cell_setting     orthorhombic
_symmetry_space_group_name_H-M     'A b a 2'
loop_
    _symmetry_equiv_pos_as_xyz
    'x, y, z'
    '-x, -y, z'
    '-x+1/2, y, z+1/2'
    'x+1/2, -y, z+1/2'
    'x, y+1/2, z+1/2'
    '-x, -y+1/2, z+1/2'
    '-x+1/2, y+1/2, z+1'
    'x+1/2, -y+1/2, z+1'
_cell_length_a     9.1639(2)
_cell_length_b     9.9730(2)
_cell_length_c     11.1913(2)
_cell_angle_alpha     90.00
_cell_angle_beta     90.00
_cell_angle_gamma     90.00
_cell_volume     1022.79(4)
_cell_formula_units_Z     4
_cell_measurement_reflns_used     25665
_cell_measurement_theta_min     1.02
_cell_measurement_theta_max     37.78
_cell_measurement_temperature     293(2)
_exptl_crystal_description     irregular
_exptl_crystal_colour     black
_exptl_crystal_size_max      .089
_exptl_crystal_size_mid      .062
_exptl_crystal_size_min      .050
_exptl_crystal_density_diffrn     7.189
_exptl_crystal_density_meas     ?
_exptl_crystal_density_method     'not measured'
_exptl_crystal_F_000     1982
_exptl_absorpt_coefficient_mu     14.179
_exptl_absorpt_correction_type     'multi-scan'
_exptl_absorpt_process_details     '(SORTAV; Blessing, 1995)'
_exptl_absorpt_correction_T_min      .247
_exptl_absorpt_correction_T_max      .468
_diffrn_ambient_temperature     293(2)
_diffrn_radiation_type     MoK\a
_diffrn_radiation_wavelength      .71070
_diffrn_radiation_source     'fine-focus sealed tube'
_diffrn_radiation_monochromator     graphite
_diffrn_measurement_device_type     'Nonius KappaCCD'
_diffrn_measurement_device     '95mm CCD camera on κ-goniostat'
_diffrn_measurement_method     'φ scans (κ = 0) plus additional ω'
_diffrn_detector_area_resol_mean     9
_diffrn_reflns_number     11905
_diffrn_reflns_av_R_equivalents      .0457
_diffrn_reflns_av_sigmaI/netI      .0438
_diffrn_reflns_theta_min     3.53
_diffrn_reflns_theta_max     37.77
_diffrn_reflns_theta_full     37.77
_diffrn_measured_fraction_theta_max      .996
_diffrn_measured_fraction_theta_full      .996
_diffrn_reflns_limit_h_min     -15
_diffrn_reflns_limit_h_max     15
_diffrn_reflns_limit_k_min     -17
_diffrn_reflns_limit_k_max     16
_diffrn_reflns_limit_l_min     -19
_diffrn_reflns_limit_l_max     17
_diffrn_standards_number     none
_diffrn_standards_interval_count     none
_diffrn_standards_interval_time     none
_diffrn_standards_decay_%     none
_refine_special_details
;
Refinement of F² against ALL reflections.  The weighted R-factor wR and
goodness of fit S are based on F², conventional R-factors R are based
on F, with F set to zero for negative F². The threshold expression of
F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
not relevant to the choice of reflections for refinement.  R-factors based
on F² are statistically about twice as large as those based on F, and R-
factors based on ALL data will be even larger.
;
_reflns_number_total     2556
_reflns_number_gt     2388
_reflns_threshold_expression     I>2σ(I)
_refine_ls_structure_factor_coef     Fsqd
_refine_ls_matrix_type     full
_refine_ls_R_factor_all      .0391
_refine_ls_R_factor_gt      .0355
_refine_ls_wR_factor_ref      .0840
_refine_ls_goodness_of_fit_ref     1.107
_refine_ls_restrained_S_all     1.107
_refine_ls_number_reflns     2556
_refine_ls_number_parameters     109
_refine_ls_number_restraints     1
_refine_ls_hydrogen_treatment     none
_refine_ls_weighting_scheme     calc
_refine_ls_weighting_details
    'calc w = 1/[σ²(Fo²)+(0.0238P)²+32.3150P] where P = (Fo²+2Fc²)/3'
_refine_ls_shift/su_max     <0.001
_refine_ls_shift/su_mean      .000
_refine_diff_density_max     2.829
_refine_diff_density_min     -2.268
_refine_ls_extinction_method     SHELXL97
_refine_ls_extinction_coef      .00120(8)
_refine_ls_abs_structure_details     'Flack H D (1983), 1137 Friedel pairs'
_refine_ls_abs_structure_Flack      -.01(2)
loop_
    _atom_type_symbol
    _atom_type_description
    _atom_type_scat_dispersion_real
    _atom_type_scat_dispersion_imag
    _atom_type_scat_source
    'Nd' 'Nd'  -.1943 3.0179
                         'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
    'Mo' 'Mo' -1.6832  .6857
                         'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
    'O' 'O'  .0106  .0060
                         'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
_computing_data_collection     'COLLECT (Nonius, 1998)'
_computing_cell_refinement     'COLLECT'
_computing_data_reduction     'DENZO and SCALEPACK (Otwinowski & Minor, 1997)'
_computing_structure_solution     'see Experimental'
_computing_structure_refinement     'SHELXL97 (Sheldrick, 1997)'
_computing_molecular_graphics     'DIAMOND (Bergerhoff, 1996)'
_computing_publication_material     'SHELXL97'
loop_
    _atom_site_label
    _atom_site_fract_x
    _atom_site_fract_y
    _atom_site_fract_z
    _atom_site_U_iso_or_equiv
    _atom_site_adp_type
    _atom_site_calc_flag
    _atom_site_refinement_flags
    _atom_site_occupancy
    _atom_site_disorder_assembly
    _atom_site_disorder_group
    _atom_site_type_symbol
    Nd  .0000  .0000  .49956(7)  .01190(10) Uani d S 1 . . Nd
    Mo1  .12151(6)  -.07437(5)  .83767(5)  .00579(11) Uani d . 1 . . Mo
    Mo2  .11841(5)  .16082(5)  -.04131(5)  .00617(10) Uani d . 1 . . Mo
    Mo3  .12480(6)  -.08277(5)  .08093(5)  .00596(11) Uani d . 1 . . Mo
    Mo4  .12416(7)  .66309(7)  .69340(6)  .00741(17) Uani d P  .849(4) . . Mo
    O1  .2434(7)  .3313(5)  .2037(5)  .0079(8) Uani d . 1 . . O
    O2  .2470(7)  .0831(4)  .3329(5)  .0093(8) Uani d . 1 . . O
    O3  .0159(6)  .2514(5)  .3341(4)  .0072(8) Uani d . 1 . . O
    O4  .2323(5)  .3457(5)  .9562(5)  .0089(8) Uani d . 1 . . O
    O5  .2679(6)  .0795(4)  .0765(6)  .0099(9) Uani d . 1 . . O
    O6  -.0079(6)  .2616(5)  .0770(5)  .0141(10) Uani d . 1 . . O
    O7  .0000  .0000  .7132(7)  .0080(11) Uani d S 1 . . O
    O8  .0000  .0000  .2229(7)  .0121(13) Uani d S 1 . . O
_geom_special_details
;
All esds (except the esd in the dihedral angle between two l.s. planes)
are estimated using the full covariance matrix.  The cell esds are taken
into account individually in the estimation of esds in distances, angles
and torsion angles; correlations between esds in cell parameters are only
used when they are defined by crystal symmetry.  An approximate (isotropic)
treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
    _geom_bond_atom_site_label_1
    _geom_bond_atom_site_label_2
    _geom_bond_site_symmetry_2
    _geom_bond_distance
    _geom_bond_publ_flag
    Nd O7 . 2.391(7) Y
    Nd O5 3 2.428(5) Y
    Nd O5 4_455 2.428(5) Y
    Nd O6 6 2.531(6) Y
    Nd O6 5_545 2.531(6) y
    Nd O4 6_554 2.671(5) Y
    Nd O4 5_544 2.671(5) Y
    Nd O2 2 3.048(6) Y
    Nd O2 . 3.048(6) Y
    Nd O8 . 3.096(8) Y
    Nd O3 2 3.121(5) Y
    Nd O3 . 3.121(5) Y
    Nd Mo2 6 3.5817(5) ?
    Nd Mo2 5_545 3.5817(5) ?
    Nd Mo3 3 3.6513(6) ?
    Mo1 O7 . 1.931(5) y
    Mo1 O2 3 1.980(5) y
    Mo1 O3 5_545 1.989(5) y
    Mo1 O4 7_544 2.047(5) y
    Mo1 O1 5_545 2.093(6) y
    Mo1 Mo1 2 2.6758(11) y
    Mo1 Mo2 1_556 2.7086(7) y
    Mo1 Mo2 2_556 2.7223(7) y
    Mo1 Mo3 1_556 2.7238(8) y
    Mo1 Mo4 1_545 3.0761(8) y
    Mo1 Mo4 7_544 3.6942(8) ?
    Mo1 Mo3 3 3.6969(7) ?
    Mo1 Nd 3 3.9828(6) ?
    Mo2 O6 . 2.025(5) y
    Mo2 O2 3_554 2.026(6) y
    Mo2 O3 6_554 2.055(5) y
    Mo2 O5 . 2.067(6) y
    Mo2 O4 1_554 2.119(5) y
    Mo2 Mo4 5_544 2.6274(9) y
    Mo2 Mo1 1_554 2.7086(7) ?
    Mo2 Mo1 2_554 2.7223(7) ?
    Mo2 Mo3 2 2.7286(7) y
    Mo2 Mo3 . 2.7886(7) y
    Mo2 Nd 5_554 3.5817(5) ?
    Mo2 Nd 3_554 3.8742(5) ?
    Mo3 O1 7_544 2.021(6) y
    Mo3 O4 7_543 2.042(5) y
    Mo3 O6 2 2.082(5) y
    Mo3 O5 . 2.083(5) y
    Mo3 O8 . 2.125(6) y
    Mo3 Mo1 1_554 2.7238(8) ?
    Mo3 Mo4 6_554 2.7261(9) y
    Mo3 Mo2 2 2.7286(7) ?
    Mo3 Mo4 5_544 2.7562(8) y
    Mo3 Mo3 2 2.8209(10) y
    Mo3 Mo4 3_544 3.6469(8) ?
    Mo3 Nd 3_554 3.6513(6) ?
    Mo3 Mo1 3_554 3.6969(7) ?
    Mo4 O1 5 2.005(5) y
    Mo4 O8 5 2.0123(15) y
    Mo4 O6 5 2.032(6) y
    Mo4 O5 5 2.035(6) y
    Mo4 O3 5 2.059(5) y
    Mo4 O2 5 2.084(6) y
    Mo4 Mo2 5 2.6274(9) ?
    Mo4 Mo3 6 2.7261(9) ?
    Mo4 Mo3 5 2.7562(8) ?
    Mo4 Mo1 1_565 3.0761(8) ?
    Mo4 Mo3 3_565 3.6469(8) ?
    Mo4 Mo1 7_554 3.6942(8) ?
    Mo4 Nd 5 3.9598(9) ?
    O1 Mo4 5_544 2.005(5) ?
    O1 Mo3 7_554 2.021(6) ?
    O1 Mo1 5_554 2.093(5) ?
    O2 Mo1 3_554 1.980(5) ?
    O2 Mo2 3 2.026(6) ?
    O2 Mo4 5_544 2.084(6) ?
    O3 Mo1 5_554 1.989(5) ?
    O3 Mo2 6 2.055(5) ?
    O3 Mo4 5_544 2.059(5) ?
    O4 Mo3 7 2.042(5) ?
    O4 Mo1 7_554 2.047(5) ?
    O4 Mo2 1_556 2.119(5) ?
    O4 Nd 5 2.671(5) ?
    O5 Mo4 5_544 2.035(6) ?
    O5 Nd 3_554 2.428(5) ?
    O6 Mo4 5_544 2.032(6) ?
    O6 Mo3 2 2.082(5) ?
    O6 Nd 5_554 2.531(6) ?
    O7 Mo1 2 1.931(5) ?
    O8 Mo4 6_554 2.0123(15) ?
    O8 Mo4 5_544 2.0123(15) ?
    O8 Mo3 2 2.125(6) ?
loop_
    _geom_angle_atom_site_label_1
    _geom_angle_atom_site_label_2
    _geom_angle_atom_site_label_3
    _geom_angle_site_symmetry_1
    _geom_angle_site_symmetry_3
    _geom_angle
    _geom_angle_publ_flag
    O7 Nd O5 . 3 69.23(15) ?
    O7 Nd O5 . 4_455 69.23(15) ?
    O5 Nd O5 3 4_455 138.5(3) ?
    O7 Nd O6 . 6 69.99(12) ?
    O5 Nd O6 3 6 63.06(16) ?
    O5 Nd O6 4_455 6 102.14(17) ?
    O7 Nd O6 . 5_545 69.99(12) ?
    O5 Nd O6 3 5_545 102.14(17) ?
    O5 Nd O6 4_455 5_545 63.06(16) ?
    O6 Nd O6 6 5_545 140.0(2) ?
    O7 Nd O4 . 6_554 100.46(13) ?
    O5 Nd O4 3 6_554 125.07(14) ?
    O5 Nd O4 4_455 6_554 63.53(15) ?
    O6 Nd O4 6 6_554 62.86(17) ?
    O6 Nd O4 5_545 6_554 125.48(17) ?
    O7 Nd O4 . 5_544 100.46(13) ?
    O5 Nd O4 3 5_544 63.53(15) ?
    O5 Nd O4 4_455 5_544 125.07(14) ?
    O6 Nd O4 6 5_544 125.48(17) ?
    O6 Nd O4 5_545 5_544 62.86(17) ?
    O4 Nd O4 6_554 5_544 159.1(3) ?
    O7 Nd O2 . 2 127.73(12) ?
    O5 Nd O2 3 2 163.0(2) ?
    O5 Nd O2 4_455 2 58.50(16) ?
    O6 Nd O2 6 2 119.07(16) ?
    O6 Nd O2 5_545 2 86.15(16) ?
    O4 Nd O2 6_554 2 56.88(13) ?
    O4 Nd O2 5_544 2 108.92(16) ?
    O7 Nd O2 . . 127.73(12) ?
    O5 Nd O2 3 . 58.50(16) ?
    O5 Nd O2 4_455 . 163.0(2) ?
    O6 Nd O2 6 . 86.15(16) ?
    O6 Nd O2 5_545 . 119.07(16) ?
    O4 Nd O2 6_554 . 108.92(16) ?
    O4 Nd O2 5_544 . 56.88(13) ?
    O2 Nd O2 2 . 104.5(2) ?
    O7 Nd O8 . . 180.0000(10)
                            ?
    O5 Nd O8 3 . 110.77(15) ?
    O5 Nd O8 4_455 . 110.77(15) ?
    O6 Nd O8 6 . 110.01(12) ?
    O6 Nd O8 5_545 . 110.01(12) ?
    O4 Nd O8 6_554 . 79.54(13) ?
    O4 Nd O8 5_544 . 79.54(13) ?
    O2 Nd O8 2 . 52.27(11) ?
    O2 Nd O8 . . 52.27(11) ?
    O7 Nd O3 . 2 126.40(9) ?
    O5 Nd O3 3 2 120.91(16) ?
    O5 Nd O3 4_455 2 84.67(16) ?
    O6 Nd O3 6 2 163.56(16) ?
    O6 Nd O3 5_545 2 56.43(14) ?
    O4 Nd O3 6_554 2 108.54(15) ?
    O4 Nd O3 5_544 2 57.77(14) ?
    O2 Nd O3 2 2 51.95(14) ?
    O2 Nd O3 . 2 83.69(13) ?
    O8 Nd O3 . 2 53.60(9) ?
    O7 Nd O3 . . 126.40(9) ?
    O5 Nd O3 3 . 84.67(15) ?
    O5 Nd O3 4_455 . 120.91(16) ?
    O6 Nd O3 6 . 56.43(14) ?
    O6 Nd O3 5_545 . 163.56(16) ?
    O4 Nd O3 6_554 . 57.77(14) ?
    O4 Nd O3 5_544 . 108.54(14) ?
    O2 Nd O3 2 . 83.69(13) ?
    O2 Nd O3 . . 51.95(14) ?
    O8 Nd O3 . . 53.60(9) ?
    O3 Nd O3 2 . 107.21(18) ?
    O7 Nd Mo2 . 6 97.338(16) ?
    O5 Nd Mo2 3 6 90.13(11) ?
    O5 Nd Mo2 4_455 6 95.06(11) ?
    O6 Nd Mo2 6 6 33.42(12) ?
    O6 Nd Mo2 5_545 6 157.23(12) ?
    O4 Nd Mo2 6_554 6 36.03(10) ?
    O4 Nd Mo2 5_544 6 139.67(11) ?
    O2 Nd Mo2 2 6 87.34(9) ?
    O2 Nd Mo2 . 6 83.69(9) ?
    O8 Nd Mo2 . 6 82.662(16) ?
    O3 Nd Mo2 2 6 131.99(9) ?
    O3 Nd Mo2 . 6 34.86(10) ?
    O7 Nd Mo2 . 5_545 97.338(16) ?
    O5 Nd Mo2 3 5_545 95.06(11) ?
    O5 Nd Mo2 4_455 5_545 90.13(11) ?
    O6 Nd Mo2 6 5_545 157.23(13) ?
    O6 Nd Mo2 5_545 5_545 33.42(12) ?
    O4 Nd Mo2 6_554 5_545 139.67(11) ?
    O4 Nd Mo2 5_544 5_545 36.03(10) ?
    O2 Nd Mo2 2 5_545 83.69(9) ?
    O2 Nd Mo2 . 5_545 87.34(9) ?
    O8 Nd Mo2 . 5_545 82.662(16) ?
    O3 Nd Mo2 2 5_545 34.86(10) ?
    O3 Nd Mo2 . 5_545 131.99(9) ?
    Mo2 Nd Mo2 6 5_545 165.32(3) ?
    O7 Nd Mo3 . 3 75.558(14) ?
    O5 Nd Mo3 3 3 32.90(11) ?
    O5 Nd Mo3 4_455 3 131.51(13) ?
    O6 Nd Mo3 6 3 95.75(13) ?
    O6 Nd Mo3 5_545 3 74.29(14) ?
    O4 Nd Mo3 6_554 3 157.82(10) ?
    O4 Nd Mo3 5_544 3 33.34(12) ?
    O2 Nd Mo3 2 3 142.23(10) ?
    O2 Nd Mo3 . 3 60.97(11) ?
    O8 Nd Mo3 . 3 104.442(14) ?
    O3 Nd Mo3 2 3 90.59(10) ?
    O3 Nd Mo3 . 3 106.60(9) ?
    Mo2 Nd Mo3 6 3 122.047(11) ?
    Mo2 Nd Mo3 5_545 3 62.166(11) ?
    O7 Mo1 O2 . 3 91.54(18) ?
    O7 Mo1 O3 . 5_545 92.32(15) ?
    O2 Mo1 O3 3 5_545 171.2(2) ?
    O7 Mo1 O4 . 7_544 173.9(2) ?
    O2 Mo1 O4 3 7_544 85.9(2) ?
    O3 Mo1 O4 5_545 7_544 89.5(2) ?
    O7 Mo1 O1 . 5_545 87.9(2) ?
    O2 Mo1 O1 3 5_545 90.7(2) ?
    O3 Mo1 O1 5_545 5_545 81.5(2) ?
    O4 Mo1 O1 7_544 5_545 86.6(2) ?
    O7 Mo1 Mo1 . 2 46.16(15) ?
    O2 Mo1 Mo1 3 2 93.83(17) ?
    O3 Mo1 Mo1 5_545 2 94.55(15) ?
    O4 Mo1 Mo1 7_544 2 139.51(16) ?
    O1 Mo1 Mo1 5_545 2 133.90(16) ?
    O7 Mo1 Mo2 . 1_556 91.26(11) ?
    O2 Mo1 Mo2 3 1_556 48.17(17) ?
    O3 Mo1 Mo2 5_545 1_556 139.58(15) ?
    O4 Mo1 Mo2 7_544 1_556 91.14(14) ?
    O1 Mo1 Mo2 5_545 1_556 138.85(15) ?
    Mo1 Mo1 Mo2 2 1_556 60.74(2) ?
    O7 Mo1 Mo2 . 2_556 90.85(11) ?
    O2 Mo1 Mo2 3 2_556 139.11(17) ?
    O3 Mo1 Mo2 5_545 2_556 48.73(15) ?
    O4 Mo1 Mo2 7_544 2_556 94.74(15) ?
    O1 Mo1 Mo2 5_545 2_556 130.17(15) ?
    Mo1 Mo1 Mo2 2 2_556 60.23(2) ?
    Mo2 Mo1 Mo2 1_556 2_556 90.98(3) ?
    O7 Mo1 Mo3 . 1_556 137.65(15) ?
    O2 Mo1 Mo3 3 1_556 92.55(18) ?
    O3 Mo1 Mo3 5_545 1_556 89.92(15) ?
    O4 Mo1 Mo3 7_544 1_556 48.16(16) ?
    O1 Mo1 Mo3 5_545 1_556 134.12(16) ?
    Mo1 Mo1 Mo3 2 1_556 91.505(16) ?
    Mo2 Mo1 Mo3 1_556 1_556 61.771(19) ?
    Mo2 Mo1 Mo3 2_556 1_556 60.13(2) ?
    O7 Mo1 Mo4 . 1_545 87.30(11) ?
    O2 Mo1 Mo4 3 1_545 131.00(17) ?
    O3 Mo1 Mo4 5_545 1_545 41.40(15) ?
    O4 Mo1 Mo4 7_544 1_545 90.21(14) ?
    O1 Mo1 Mo4 5_545 1_545 40.29(14) ?
    Mo1 Mo1 Mo4 2 1_545 118.58(3) ?
    Mo2 Mo1 Mo4 1_556 1_545 178.33(3) ?
    Mo2 Mo1 Mo4 2_556 1_545 89.88(2) ?
    Mo3 Mo1 Mo4 1_556 1_545 119.89(2) ?
    O7 Mo1 Mo4 . 7_544 78.60(7) ?
    O2 Mo1 Mo4 3 7_544 25.30(18) ?
    O3 Mo1 Mo4 5_545 7_544 149.10(15) ?
    O4 Mo1 Mo4 7_544 7_544 96.90(14) ?
    O1 Mo1 Mo4 5_545 7_544 68.80(14) ?
    Mo1 Mo1 Mo4 2 7_544 99.77(3) ?
    Mo2 Mo1 Mo4 1_556 7_544 70.731(19) ?
    Mo2 Mo1 Mo4 2_556 7_544 158.43(2) ?
    Mo3 Mo1 Mo4 1_556 7_544 116.71(2) ?
    Mo4 Mo1 Mo4 1_545 7_544 108.13(2) ?
    O7 Mo1 Mo3 . 3 79.09(14) ?
    O2 Mo1 Mo3 3 3 67.32(17) ?
    O3 Mo1 Mo3 5_545 3 105.70(15) ?
    O4 Mo1 Mo3 7_544 3 94.79(16) ?
    O1 Mo1 Mo3 5_545 3 25.51(13) ?
    Mo1 Mo1 Mo3 2 3 122.405(16) ?
    Mo2 Mo1 Mo3 1_556 3 114.51(2) ?
    Mo2 Mo1 Mo3 2_556 3 152.54(2) ?
    Mo3 Mo1 Mo3 1_556 3 140.27(2) ?
    Mo4 Mo1 Mo3 1_545 3 64.394(17) ?
    Mo4 Mo1 Mo3 7_544 3 43.789(14) ?
    O7 Mo1 Nd . 3 139.34(4) ?
    O2 Mo1 Nd 3 3 48.29(17) ?
    O3 Mo1 Nd 5_545 3 126.55(15) ?
    O4 Mo1 Nd 7_544 3 37.61(14) ?
    O1 Mo1 Nd 5_545 3 86.83(17) ?
    Mo1 Mo1 Nd 2 3 128.43(2) ?
    Mo2 Mo1 Nd 1_556 3 67.692(15) ?
    Mo2 Mo1 Nd 2_556 3 122.41(2) ?
    Mo3 Mo1 Nd 1_556 3 62.704(18) ?
    Mo4 Mo1 Nd 1_545 3 112.98(2) ?
    Mo4 Mo1 Nd 7_544 3 61.967(15) ?
    Mo3 Mo1 Nd 3 3 79.055(16) ?
    O7 Mo1 Nd . . 24.37(15) ?
    O2 Mo1 Nd 3 . 89.82(18) ?
    O3 Mo1 Nd 5_545 . 90.43(14) ?
    O4 Mo1 Nd 7_544 . 149.84(16) ?
    O1 Mo1 Nd 5_545 . 63.63(16) ?
    Mo1 Mo1 Nd 2 . 70.528(8) ?
    Mo2 Mo1 Nd 1_556 . 107.97(2) ?
    Mo2 Mo1 Nd 2_556 . 107.667(19) ?
    Mo3 Mo1 Nd 1_556 . 162.00(2) ?
    Mo4 Mo1 Nd 1_545 . 70.406(16) ?
    Mo4 Mo1 Nd 7_544 . 69.176(14) ?
    Mo3 Mo1 Nd 3 . 56.351(12) ?
    Nd Mo1 Nd 3 . 129.499(17) ?
    O6 Mo2 O2 . 3_554 172.7(2) ?
    O6 Mo2 O3 . 6_554 83.7(2) ?
    O2 Mo2 O3 3_554 6_554 93.2(2) ?
    O6 Mo2 O5 . . 99.0(2) ?
    O2 Mo2 O5 3_554 . 83.7(2) ?
    O3 Mo2 O5 6_554 . 175.27(19) ?
    O6 Mo2 O4 . 1_554 81.8(2) ?
    O2 Mo2 O4 3_554 1_554 91.4(2) ?
    O3 Mo2 O4 6_554 1_554 85.2(2) ?
    O5 Mo2 O4 . 1_554 91.33(19) ?
    O6 Mo2 Mo4 . 5_544 49.75(18) ?
    O2 Mo2 Mo4 3_554 5_544 133.30(18) ?
    O3 Mo2 Mo4 6_554 5_544 133.36(15) ?
    O5 Mo2 Mo4 . 5_544 49.64(17) ?
    O4 Mo2 Mo4 1_554 5_544 89.74(16) ?
    O6 Mo2 Mo1 . 1_554 139.70(15) ?
    O2 Mo2 Mo1 3_554 1_554 46.75(15) ?
    O3 Mo2 Mo1 6_554 1_554 92.05(15) ?
    O5 Mo2 Mo1 . 1_554 88.41(14) ?
    O4 Mo2 Mo1 1_554 1_554 137.89(15) ?
    Mo4 Mo2 Mo1 5_544 1_554 120.47(3) ?
    O6 Mo2 Mo1 . 2_554 91.20(17) ?
    O2 Mo2 Mo1 3_554 2_554 91.42(18) ?
    O3 Mo2 Mo1 6_554 2_554 46.66(14) ?
    O5 Mo2 Mo1 . 2_554 136.74(13) ?
    O4 Mo2 Mo1 1_554 2_554 131.84(15) ?
    Mo4 Mo2 Mo1 5_544 2_554 121.08(3) ?
    Mo1 Mo2 Mo1 1_554 2_554 59.03(2) ?
    O6 Mo2 Mo3 . 2 49.25(15) ?
    O2 Mo2 Mo3 3_554 2 137.44(15) ?
    O3 Mo2 Mo3 6_554 2 88.42(14) ?
    O5 Mo2 Mo3 . 2 96.29(16) ?
    O4 Mo2 Mo3 1_554 2 131.08(14) ?
    Mo4 Mo2 Mo3 5_544 2 61.16(2) ?
    Mo1 Mo2 Mo3 1_554 2 90.70(2) ?
    Mo1 Mo2 Mo3 2_554 2 59.960(19) ?
    O6 Mo2 Mo3 . . 97.12(16) ?
    O2 Mo2 Mo3 3_554 . 89.70(13) ?
    O3 Mo2 Mo3 6_554 . 135.74(14) ?
    O5 Mo2 Mo3 . . 48.04(13) ?
    O4 Mo2 Mo3 1_554 . 138.94(15) ?
    Mo4 Mo2 Mo3 5_544 . 61.09(2) ?
    Mo1 Mo2 Mo3 1_554 . 59.382(18) ?
    Mo1 Mo2 Mo3 2_554 . 89.15(2) ?
    Mo3 Mo2 Mo3 2 . 61.49(2) ?
    O6 Mo2 Nd . 5_554 43.50(16) ?
    O2 Mo2 Nd 3_554 5_554 129.39(13) ?
    O3 Mo2 Nd 6_554 5_554 60.21(15) ?
    O5 Mo2 Nd . 5_554 119.33(14) ?
    O4 Mo2 Nd 1_554 5_554 47.87(13) ?
    Mo4 Mo2 Nd 5_544 5_554 82.54(2) ?
    Mo1 Mo2 Nd 1_554 5_554 152.23(3) ?
    Mo1 Mo2 Nd 2_554 5_554 96.774(19) ?
    Mo3 Mo2 Nd 2 5_554 87.589(18) ?
    Mo3 Mo2 Nd . 5_554 140.03(2) ?
    O6 Mo2 Nd . 3_554 130.09(18) ?
    O2 Mo2 Nd 3_554 3_554 51.25(18) ?
    O3 Mo2 Nd 6_554 3_554 142.83(14) ?
    O5 Mo2 Nd . 3_554 33.29(17) ?
    O4 Mo2 Nd 1_554 3_554 85.24(13) ?
    Mo4 Mo2 Nd 5_544 3_554 82.38(2) ?
    Mo1 Mo2 Nd 1_554 3_554 72.006(16) ?
    Mo1 Mo2 Nd 2_554 3_554 131.04(2) ?
    Mo3 Mo2 Nd 2 3_554 124.05(2) ?
    Mo3 Mo2 Nd . 3_554 64.054(16) ?
    Nd Mo2 Nd 5_554 3_554 130.491(16) ?
    O1 Mo3 O4 7_544 7_543 86.2(2) ?
    O1 Mo3 O6 7_544 2 87.6(2) ?
    O4 Mo3 O6 7_543 2 90.9(2) ?
    O1 Mo3 O5 7_544 . 88.3(2) ?
    O4 Mo3 O5 7_543 . 81.5(2) ?
    O6 Mo3 O5 2 . 171.6(2) ?
    O1 Mo3 O8 7_544 . 88.7(2) ?
    O4 Mo3 O8 7_543 . 172.69(18) ?
    O6 Mo3 O8 2 . 94.12(18) ?
    O5 Mo3 O8 . . 93.14(16) ?
    O1 Mo3 Mo1 7_544 1_554 134.39(16) ?
    O4 Mo3 Mo1 7_543 1_554 48.31(15) ?
    O6 Mo3 Mo1 2 1_554 89.96(16) ?
    O5 Mo3 Mo1 . 1_554 87.67(18) ?
    O8 Mo3 Mo1 . 1_554 136.85(14) ?
    O1 Mo3 Mo4 7_544 6_554 93.53(17) ?
    O4 Mo3 Mo4 7_543 6_554 138.54(14) ?
    O6 Mo3 Mo4 2 6_554 47.71(18) ?
    O5 Mo3 Mo4 . 6_554 139.99(16) ?
    O8 Mo3 Mo4 . 6_554 47.03(2) ?
    Mo1 Mo3 Mo4 1_554 6_554 117.47(3) ?
    O1 Mo3 Mo2 7_544 2 135.10(15) ?
    O4 Mo3 Mo2 7_543 2 94.67(15) ?
    O6 Mo3 Mo2 2 2 47.49(15) ?
    O5 Mo3 Mo2 . 2 136.36(16) ?
    O8 Mo3 Mo2 . 2 92.64(10) ?
    Mo1 Mo3 Mo2 1_554 2 59.906(19) ?
    Mo4 Mo3 Mo2 6_554 2 57.59(2) ?
    O1 Mo3 Mo4 7_544 5_544 93.90(14) ?
    O4 Mo3 Mo4 7_543 5_544 128.63(14) ?
    O6 Mo3 Mo4 2 5_544 140.45(18) ?
    O5 Mo3 Mo4 . 5_544 47.25(16) ?
    O8 Mo3 Mo4 . 5_544 46.50(2) ?
    Mo1 Mo3 Mo4 1_554 5_544 115.41(3) ?
    Mo4 Mo3 Mo4 6_554 5_544 92.80(3) ?
    Mo2 Mo3 Mo4 2 5_544 118.75(2) ?
    O1 Mo3 Mo2 7_544 . 135.71(15) ?
    O4 Mo3 Mo2 7_543 . 89.00(14) ?
    O6 Mo3 Mo2 2 . 136.49(15) ?
    O5 Mo3 Mo2 . . 47.53(15) ?
    O8 Mo3 Mo2 . . 90.98(10) ?
    Mo1 Mo3 Mo2 1_554 . 58.847(18) ?
    Mo4 Mo3 Mo2 6_554 . 117.71(3) ?
    Mo2 Mo3 Mo2 2 . 89.16(2) ?
    Mo4 Mo3 Mo2 5_544 . 56.57(2) ?
    O1 Mo3 Mo3 7_544 2 137.14(16) ?
    O4 Mo3 Mo3 7_543 2 136.41(15) ?
    O6 Mo3 Mo3 2 2 94.82(17) ?
    O5 Mo3 Mo3 . 2 93.19(14) ?
    O8 Mo3 Mo3 . 2 48.40(14) ?
    Mo1 Mo3 Mo3 1_554 2 88.454(15) ?
    Mo4 Mo3 Mo3 6_554 2 59.56(2) ?
    Mo2 Mo3 Mo3 2 2 60.30(2) ?
    Mo4 Mo3 Mo3 5_544 2 58.51(2) ?
    Mo2 Mo3 Mo3 . 2 58.207(17) ?
    O1 Mo3 Mo4 7_544 3_544 24.95(14) ?
    O4 Mo3 Mo4 7_543 3_544 65.71(15) ?
    O6 Mo3 Mo4 2 3_544 74.72(16) ?
    O5 Mo3 Mo4 . 3_544 98.69(14) ?
    O8 Mo3 Mo4 . 3_544 110.58(14) ?
    Mo1 Mo3 Mo4 1_554 3_544 111.92(2) ?
    Mo4 Mo3 Mo4 6_554 3_544 99.46(2) ?
    Mo2 Mo3 Mo4 2 3_544 119.34(2) ?
    Mo4 Mo3 Mo4 5_544 3_544 117.52(2) ?
    Mo2 Mo3 Mo4 . 3_544 142.00(2) ?
    Mo3 Mo3 Mo4 2 3_544 156.66(2) ?
    O1 Mo3 Nd 7_544 3_554 72.70(17) ?
    O4 Mo3 Nd 7_543 3_554 45.96(14) ?
    O6 Mo3 Nd 2 3_554 132.31(18) ?
    O5 Mo3 Nd . 3_554 39.27(15) ?
    O8 Mo3 Nd . 3_554 127.27(6) ?
    Mo1 Mo3 Nd 1_554 3_554 75.77(2) ?
    Mo4 Mo3 Nd 6_554 3_554 165.85(3) ?
    Mo2 Mo3 Nd 2 3_554 135.12(2) ?
    Mo4 Mo3 Nd 5_544 3_554 85.112(19) ?
    Mo2 Mo3 Nd . 3_554 72.573(16) ?
    Mo3 Mo3 Nd 2 3_554 129.14(2) ?
    Mo4 Mo3 Nd 3_544 3_554 69.464(16) ?
    O1 Mo3 Mo1 7_544 3_554 26.49(13) ?
    O4 Mo3 Mo1 7_543 3_554 97.81(15) ?
    O6 Mo3 Mo1 2 3_554 111.08(15) ?
    O5 Mo3 Mo1 . 3_554 66.75(16) ?
    O8 Mo3 Mo1 . 3_554 75.43(13) ?
    Mo1 Mo3 Mo1 1_554 3_554 141.54(2) ?
    Mo4 Mo3 Mo1 6_554 3_554 100.03(2) ?
    Mo2 Mo3 Mo1 2 3_554 155.48(2) ?
    Mo4 Mo3 Mo1 5_544 3_554 68.053(19) ?
    Mo2 Mo3 Mo1 . 3_554 112.01(2) ?
    Mo3 Mo3 Mo1 2 3_554 119.779(15) ?
    Mo4 Mo3 Mo1 3_544 3_554 49.521(15) ?
    Nd Mo3 Mo1 3_554 3_554 66.207(16) ?
    O1 Mo4 O8 5 5 167.1(3) ?
    O1 Mo4 O6 5 5 87.5(2) ?
    O8 Mo4 O6 5 5 99.2(2) ?
    O1 Mo4 O5 5 5 91.6(2) ?
    O8 Mo4 O5 5 5 98.06(19) ?
    O6 Mo4 O5 5 5 99.9(2) ?
    O1 Mo4 O3 5 5 82.0(2) ?
    O8 Mo4 O3 5 5 87.0(2) ?
    O6 Mo4 O3 5 5 89.8(2) ?
    O5 Mo4 O3 5 5 168.2(2) ?
    O1 Mo4 O2 5 5 89.0(2) ?
    O8 Mo4 O2 5 5 82.7(2) ?
    O6 Mo4 O2 5 5 171.0(2) ?
    O5 Mo4 O2 5 5 88.6(2) ?
    O3 Mo4 O2 5 5 81.4(2) ?
    O1 Mo4 Mo2 5 5 94.35(16) ?
    O8 Mo4 Mo2 5 5 98.4(2) ?
    O6 Mo4 Mo2 5 5 49.53(15) ?
    O5 Mo4 Mo2 5 5 50.70(16) ?
    O3 Mo4 Mo2 5 5 139.34(15) ?
    O2 Mo4 Mo2 5 5 139.17(17) ?
    O1 Mo4 Mo3 5 6 136.76(16) ?
    O8 Mo4 Mo3 5 6 50.58(16) ?
    O6 Mo4 Mo3 5 6 49.28(15) ?
    O5 Mo4 Mo3 5 6 97.14(15) ?
    O3 Mo4 Mo3 5 6 94.34(14) ?
    O2 Mo4 Mo3 5 6 133.29(15) ?
    Mo2 Mo4 Mo3 5 6 61.25(2) ?
    O1 Mo4 Mo3 5 5 140.30(17) ?
    O8 Mo4 Mo3 5 5 49.99(16) ?
    O6 Mo4 Mo3 5 5 97.97(15) ?
    O5 Mo4 Mo3 5 5 48.74(13) ?
    O3 Mo4 Mo3 5 5 136.97(15) ?
    O2 Mo4 Mo3 5 5 90.02(14) ?
    Mo2 Mo4 Mo3 5 5 62.34(2) ?
    Mo3 Mo4 Mo3 6 5 61.93(2) ?
    O1 Mo4 Mo1 5 1_565 42.44(16) ?
    O8 Mo4 Mo1 5 1_565 126.69(18) ?
    O6 Mo4 Mo1 5 1_565 85.42(15) ?
    O5 Mo4 Mo1 5 1_565 133.73(14) ?
    O3 Mo4 Mo1 5 1_565 39.70(14) ?
    O2 Mo4 Mo1 5 1_565 86.38(14) ?
    Mo2 Mo4 Mo1 5 1_565 122.14(3) ?
    Mo3 Mo4 Mo1 6 1_565 119.07(3) ?
    Mo3 Mo4 Mo1 5 1_565 175.50(3) ?
    O1 Mo4 Mo3 5 3_565 25.16(16) ?
    O8 Mo4 Mo3 5 3_565 167.17(19) ?
    O6 Mo4 Mo3 5 3_565 79.52(15) ?
    O5 Mo4 Mo3 5 3_565 69.79(13) ?
    O3 Mo4 Mo3 5 3_565 105.69(14) ?
    O2 Mo4 Mo3 5 3_565 100.60(16) ?
    Mo2 Mo4 Mo3 5 3_565 70.95(2) ?
    Mo3 Mo4 Mo3 6 3_565 124.95(3) ?
    Mo3 Mo4 Mo3 5 3_565 117.34(3) ?
    Mo1 Mo4 Mo3 1_565 3_565 66.085(18) ?
    O1 Mo4 Mo1 5 7_554 99.63(17) ?
    O8 Mo4 Mo1 5 7_554 76.52(9) ?
    O6 Mo4 Mo1 5 7_554 165.04(15) ?
    O5 Mo4 Mo1 5 7_554 67.05(16) ?
    O3 Mo4 Mo1 5 7_554 104.13(15) ?
    O2 Mo4 Mo1 5 7_554 23.96(15) ?
    Mo2 Mo4 Mo1 5 7_554 116.36(3) ?
    Mo3 Mo4 Mo1 6 7_554 122.78(3) ?
    Mo3 Mo4 Mo1 5 7_554 68.158(18) ?
    Mo1 Mo4 Mo1 1_565 7_554 108.74(2) ?
    Mo3 Mo4 Mo1 3_565 7_554 101.44(2) ?
    O1 Mo4 Nd 5 5 116.76(16) ?
    O8 Mo4 Nd 5 5 50.5(2) ?
    O6 Mo4 Nd 5 5 125.63(15) ?
    O5 Mo4 Nd 5 5 125.03(15) ?
    O3 Mo4 Nd 5 5 51.37(15) ?
    O2 Mo4 Nd 5 5 49.43(18) ?
    Mo2 Mo4 Nd 5 5 148.84(3) ?
    Mo3 Mo4 Nd 6 5 92.20(2) ?
    Mo3 Mo4 Nd 5 5 91.74(2) ?
    Mo1 Mo4 Nd 1_565 5 83.868(19) ?
    Mo3 Mo4 Nd 3_565 5 139.94(2) ?
    Mo1 Mo4 Nd 7_554 5 62.599(13) ?
    Mo4 O1 Mo3 5_544 7_554 129.9(3) ?
    Mo4 O1 Mo1 5_544 5_554 97.3(3) ?
    Mo3 O1 Mo1 7_554 5_554 128.0(2) ?
    Mo1 O2 Mo2 3_554 3 85.1(2) ?
    Mo1 O2 Mo4 3_554 5_544 130.7(3) ?
    Mo2 O2 Mo4 3 5_544 134.7(2) ?
    Mo1 O2 Nd 3_554 . 102.70(19) ?
    Mo2 O2 Nd 3 . 97.5(2) ?
    Mo4 O2 Nd 5_544 . 99.3(2) ?
    Mo1 O3 Mo2 5_554 6 84.60(19) ?
    Mo1 O3 Mo4 5_554 5_544 98.9(2) ?
    Mo2 O3 Mo4 6 5_544 171.7(3) ?
    Mo1 O3 Nd 5_554 . 135.5(2) ?
    Mo2 O3 Nd 6 . 84.93(17) ?
    Mo4 O3 Nd 5_544 . 97.61(19) ?
    Mo3 O4 Mo1 7 7_554 83.54(18) ?
    Mo3 O4 Mo2 7 1_556 127.7(3) ?
    Mo1 O4 Mo2 7_554 1_556 132.0(3) ?
    Mo3 O4 Nd 7 5 100.7(2) ?
    Mo1 O4 Nd 7_554 5 114.5(2) ?
    Mo2 O4 Nd 1_556 5 96.10(18) ?
    Mo4 O5 Mo2 5_544 . 79.66(18) ?
    Mo4 O5 Mo3 5_544 . 84.0(2) ?
    Mo2 O5 Mo3 . . 84.4(2) ?
    Mo4 O5 Nd 5_544 3_554 158.2(3) ?
    Mo2 O5 Nd . 3_554 118.9(3) ?
    Mo3 O5 Nd . 3_554 107.8(2) ?
    Mo2 O6 Mo4 . 5_544 80.7(2) ?
    Mo2 O6 Mo3 . 2 83.26(19) ?
    Mo4 O6 Mo3 5_544 2 83.0(2) ?
    Mo2 O6 Nd . 5_554 103.1(2) ?
    Mo4 O6 Nd 5_544 5_554 131.1(3) ?
    Mo3 O6 Nd 2 5_554 145.8(3) ?
    Mo1 O7 Mo1 . 2 87.7(3) ?
    Mo1 O7 Nd . . 136.16(15) ?
    Mo1 O7 Nd 2 . 136.16(15) ?
    Mo4 O8 Mo4 6_554 5_544 161.1(4) ?
    Mo4 O8 Mo3 6_554 2 83.51(18) ?
    Mo4 O8 Mo3 5_544 2 82.40(18) ?
    Mo4 O8 Mo3 6_554 . 82.40(18) ?
    Mo4 O8 Mo3 5_544 . 83.51(18) ?
    Mo3 O8 Mo3 2 . 83.2(3) ?
    Mo4 O8 Nd 6_554 . 99.4(2) ?
    Mo4 O8 Nd 5_544 . 99.4(2) ?
    Mo3 O8 Nd 2 . 138.40(14) ?
    Mo3 O8 Nd . . 138.40(14) ?
